# Superconducting scanning tunneling microscopy tips in a ... · PDF fileSuperconducting...

date post

20-Aug-2019Category

## Documents

view

217download

0

Embed Size (px)

### Transcript of Superconducting scanning tunneling microscopy tips in a ... · PDF fileSuperconducting...

Superconducting scanning tunneling microscopy tips in a magnetic field: Geometry- controlled order of the phase transition

Matthias Eltschka, , Berthold Jäck, Maximilian Assig, Oleg V. Kondrashov, Mikhail A. Skvortsov, Markus Etzkorn, Christian R. Ast, and Klaus Kern

Citation: Appl. Phys. Lett. 107, 122601 (2015); doi: 10.1063/1.4931359 View online: http://dx.doi.org/10.1063/1.4931359 View Table of Contents: http://aip.scitation.org/toc/apl/107/12 Published by the American Institute of Physics

Articles you may be interested in A nanoscale gigahertz source realized with Josephson scanning tunneling microscopy Appl. Phys. Lett. 106, 013109013109 (2015); 10.1063/1.4905322

http://oasc12039.247realmedia.com/RealMedia/ads/click_lx.ads/www.aip.org/pt/adcenter/pdfcover_test/L-37/1767098002/x01/AIP-PT/APL_ArticleDL_0117/NeedleInHaystack_1640x440.jpg/434f71374e315a556e61414141774c75?x http://aip.scitation.org/author/Eltschka%2C+Matthias http://aip.scitation.org/author/J%C3%A4ck%2C+Berthold http://aip.scitation.org/author/Assig%2C+Maximilian http://aip.scitation.org/author/Kondrashov%2C+Oleg+V http://aip.scitation.org/author/Skvortsov%2C+Mikhail+A http://aip.scitation.org/author/Etzkorn%2C+Markus http://aip.scitation.org/author/Ast%2C+Christian+R http://aip.scitation.org/author/Kern%2C+Klaus /loi/apl http://dx.doi.org/10.1063/1.4931359 http://aip.scitation.org/toc/apl/107/12 http://aip.scitation.org/publisher/ /doi/abs/10.1063/1.4905322

Superconducting scanning tunneling microscopy tips in a magnetic field: Geometry-controlled order of the phase transition

Matthias Eltschka,1,a) Berthold J€ack,1 Maximilian Assig,1 Oleg V. Kondrashov,2

Mikhail A. Skvortsov,2,3,4 Markus Etzkorn,1 Christian R. Ast,1 and Klaus Kern1,5 1Max-Planck-Institut f€ur Festk€orperforschung, 70569 Stuttgart, Germany 2Moscow Institute of Physics and Technology, 141700 Moscow, Russia 3Skolkovo Institute of Science and Technology, 143026 Moscow, Russia 4L. D. Landau Institute for Theoretical Physics, 142432 Chernogolovka, Russia 5Institut de Physique de la Matière Condens�ee, Ecole Polytechnique F�ed�erale de Lausanne, 1015 Lausanne, Switzerland

(Received 17 July 2015; accepted 7 September 2015; published online 21 September 2015)

The properties of geometrically confined superconductors significantly differ from their bulk

counterparts. Here, we demonstrate the geometrical impact for superconducting scanning tunneling

microscopy (STM) tips, where the confinement ranges from the atomic to the mesoscopic scale. To

this end, we compare the experimentally determined magnetic field dependence for several

vanadium tips to microscopic calculations based on the Usadel equation. For our theoretical model

of a superconducting cone, we find a direct correlation between the geometry and the order of the

superconducting phase transition. Increasing the opening angle of the cone changes the phase

transition from first to second order. Comparing our experimental findings to the theory reveals

first and second order quantum phase transitions in the vanadium STM tips. In addition, the theory

also explains experimentally observed broadening effects by the specific tip geometry. VC 2015 AIP Publishing LLC. [http://dx.doi.org/10.1063/1.4931359]

When geometrically confined to dimensions smaller than

the London penetration depth, superconductors in a magnetic

field exhibit properties that can significantly differ from their

bulk counterparts. For example, the critical magnetic fields, at

which superconducting thin films become normal conducting,

are considerably enhanced compared to the bulk due to geo-

metrical confinement.1–4 At the critical field, the order of the

superconducting phase transition also depends on geometrical

factors such as the film thickness.3,4 In addition to thin films,

various other geometries have been studied experimentally

and theoretically such as disks, rings, or spheres.5–10 A cone

presents a particularly interesting and challenging geometry

covering length scales from the atomic scale apex to the

macroscopic base.11 At mesoscopic length scales where super-

conductivity has to be described, cones are a highly suitable

approximation for superconducting tips in scanning tunneling

microscopy (STM). Superconducting STM tips can be

employed for enhancing the energy resolution (e. g. Refs. 12

and 13), for accessing parameters of a superconductor,14 as

probes for absolute spin polarization,15 or for designing

Josephson junctions.16–18 In a conical geometry, it is a priori not clear if the superconducting properties are affected due to

the mesoscopic confinement or if quantum size effects have

to be considered as in zero-dimensional (0D) superconduc-

tors.19–22 In this context, the magnetic field dependence of the

superconducting gap is of fundamental interest. The order of

the superconducting phase transition also remains an open

question. Therefore, it is essential to understand the impact of

the confinement on tunneling experiments employing super-

conducting STM tips.

Here, we investigate the influence of the geometry on

the superconducting phase transition of STM tips in mag-

netic fields. To this end, we measure the magnetic field de-

pendence of several vanadium tips by STM and use the

Usadel equation for modeling the tips as sharp superconduct-

ing cones in magnetic fields. Comparing our experimental

results with the calculations, we characterize the order of the

superconducting phase transitions in the V tips. We find that

we can tune the order of the phase transition by changing the

geometry of the tip apex, i.e., first order transitions for sharp

tips and second order transitions for blunt tips. Furthermore,

our approach allows to correlate experimentally observed

broadening effects to the geometric confinement of the

superconductor.

Fig. 1(a) shows differential conductance (dI/dV) tunneling spectra of a superconducting V tip on single crystal V(100) as

a function of magnetic field B and at a temperature of 15 mK.23,29 Since the critical field for bulk V Bc;bulk < 0:5 T, the sample is normal conducting for all measurements shown.

The dI/dV-spectra show the superconducting quasi-particle density of states (DOS) of the STM tip up to its critical field Bc of about 4.2 T, which is higher than in the bulk due to the

dimensional confinement near the apex.15 The lifted spin

degeneracy results in the characteristic four-peak-structure of

the superconducting coherence peaks.24

To characterize our data, we start with the simplest 0D

model of a small superconductor in a magnetic field. In this

model analyzed by Maki,25,26 the DOS is given by

q#"ðEÞ ¼ ðq0=2ÞsgnðEÞRe �

u6

. ffiffiffiffiffiffiffiffiffiffiffiffiffiffi u26 � 1

q � ; (1)

where uþ and u� are implicitly defined by

a)Author to whom correspondence should be addressed. Electronic mail:

m.eltschka@fkf.mpg.de

0003-6951/2015/107(12)/122601/5/$30.00 VC 2015 AIP Publishing LLC107, 122601-1

APPLIED PHYSICS LETTERS 107, 122601 (2015)

http://dx.doi.org/10.1063/1.4931359 http://dx.doi.org/10.1063/1.4931359 http://dx.doi.org/10.1063/1.4931359 mailto:m.eltschka@fkf.mpg.de http://crossmark.crossref.org/dialog/?doi=10.1063/1.4931359&domain=pdf&date_stamp=2015-09-21

u6 ¼ E� iCð Þ7lBB

D þ f u6ffiffiffiffiffiffiffiffiffiffiffiffiffiffi

1� u26 p þ b u7 � u6ffiffiffiffiffiffiffiffiffiffiffiffiffiffi

1� u27 p ; (2)

with q0 is the normal conducting DOS, E is the energy, lB is the magnetic moment (Bohr magneton), D is the supercon- ducting order parameter, f is the orbital depairing parameter, B is the external magnetic field, and b is the spin-orbit scat- tering parameter. In our dI/dV spectra, we usually observe broader spectral features than expected just from thermal

effects (T¼ 15 mK). At higher magnetic fields, we observe the filling of the superconducting gap where the dI/dV-signal does not completely go to zero as predicted by the original

Maki’s model.25,26 Therefore, we employ an extended

Maki’s model (EMM) with an additional phenomenological

broadening parameter C.27 Including C broadens the spectral features and results in a much better fit to our experimental

data. We emphasize that an artificially introduced parameter

C should not be attributed to any real pair-breaking mecha- nism. Its appearance is the price to pay for a good fitting of

experimental data by an oversimplified 0D Maki’s model.

Below, we present a consistent microscopic description for

our experimental data based on the Usadel equations.

In Fig. 1(a), the black solid lines represent fits to the

data using the EMM with b ¼ 0:1060:04 (which is in good agreement with Ref. 28) and a magnetic field dependent f (for details see Ref. 29). In Fig. 1(b), the same experiment is

repeated with a different V tip. While the superconducting

DOS of the tip is clearly visible and similar to Fig. 1(a), the

spectral features appear much broader and the critical field

Bc � 2:5 T is smaller. Fitting the more broadened spectra with the EMM requires larger C values than in Fig. 1(a).

Repeating these experiments for several V tips (made

from five

*View more*